#------------------------------------------------------------------------------
#$Date: 2019-11-23 12:03:07 +0200 (Sat, 23 Nov 2019) $
#$Revision: 233208 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/23/56/7235661.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7235661
loop_
_publ_author_name
'Saini, Mukesh Kumar'
'Gupta, Rakesh'
'Parbhakar, Swati'
'Kumar Mishra, Anil'
'Mathur, Rashi'
'Hussain, Firasat'
_publ_section_title
;
 Dimeric complexes of rare-earth substituted Keggin-type silicotungstates:
 syntheses, crystal structure and solid state properties
;
_journal_issue                   48
_journal_name_full               'RSC Adv.'
_journal_page_first              25357
_journal_paper_doi               10.1039/C4RA02751E
_journal_volume                  4
_journal_year                    2014
_chemical_formula_moiety         '0.5(C8 Ho4 K16 Na8 O208 Si4 W44), 6(O)'
_chemical_formula_sum            'C4 Ho2 K8 Na4 O110 Si2 W22'
_chemical_formula_weight         6643.28
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_Int_Tables_number      14
_audit_creation_date             2014-03-26
_audit_creation_method
;
Olex2 1.2
(compiled 2014.03.20 svn.r2914 for OlexSys, GUI svn.r4813)
;
_cell_angle_alpha                90
_cell_angle_beta                 110.526(4)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   20.0715(6)
_cell_length_b                   12.6297(4)
_cell_length_c                   21.0663(7)
_cell_measurement_reflns_used    19208
_cell_measurement_temperature    150.0
_cell_measurement_theta_max      29.2694
_cell_measurement_theta_min      2.8950
_cell_volume                     5001.2(3)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.34.49 (release 20-01-2011 CrysAlis171 .NET)
(compiled Jan 20 2011,15:58:25)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.34.49 (release 20-01-2011 CrysAlis171 .NET)
(compiled Jan 20 2011,15:58:25)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.34.49 (release 20-01-2011 CrysAlis171 .NET)
(compiled Jan 20 2011,15:58:25)
;
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'olex2.refine (Bourhis et al., 2013)'
_diffrn_ambient_temperature      150.0
_diffrn_detector_area_resol_mean 15.9853
_diffrn_measured_fraction_theta_full 0.9986
_diffrn_measured_fraction_theta_max 0.9986
_diffrn_measurement_device_type  'Xcalibur, Sapphire3'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_UB_11      0.0125430000
_diffrn_orient_matrix_UB_12      -0.0526498000
_diffrn_orient_matrix_UB_13      0.0008099000
_diffrn_orient_matrix_UB_21      -0.0209751000
_diffrn_orient_matrix_UB_22      -0.0158174000
_diffrn_orient_matrix_UB_23      0.0193222000
_diffrn_orient_matrix_UB_31      -0.0287459000
_diffrn_orient_matrix_UB_32      -0.0115208000
_diffrn_orient_matrix_UB_33      -0.0303135000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0570
_diffrn_reflns_av_unetI/netI     0.0520
_diffrn_reflns_limit_h_max       27
_diffrn_reflns_limit_h_min       -27
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_number            49297
_diffrn_reflns_theta_full        26.0210
_diffrn_reflns_theta_max         26.02
_diffrn_reflns_theta_min         2.90
_diffrn_source                   'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    27.244
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.18585
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.34.49 (release 20-01-2011 CrysAlis171 .NET)
(compiled Jan 20 2011,15:58:25)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'clear yellowish yellow'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   yellowish
_exptl_crystal_colour_primary    yellow
_exptl_crystal_density_diffrn    4.4113
_exptl_crystal_F_000             5763.7153
_exptl_crystal_size_max          0.14
_exptl_crystal_size_mid          0.14
_exptl_crystal_size_min          0.05
_refine_diff_density_max         6.8685
_refine_diff_density_min         -4.4940
_refine_diff_density_rms         0.9544
_refine_ls_d_res_high            0.8100
_refine_ls_d_res_low             7.0181
_refine_ls_goodness_of_fit_ref   1.0145
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     389
_refine_ls_number_reflns         9839
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.0145
_refine_ls_R_factor_all          0.0568
_refine_ls_R_factor_gt           0.0533
_refine_ls_shift/su_max          0.0052
_refine_ls_shift/su_mean         0.0003
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0161P)²+1391.7557P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1367
_refine_ls_wR_factor_ref         0.1383
_reflns_Friedel_coverage         0.0
_reflns_limit_h_max              23
_reflns_limit_h_min              -24
_reflns_limit_k_max              15
_reflns_limit_k_min              0
_reflns_limit_l_max              26
_reflns_limit_l_min              0
_reflns_number_gt                9272
_reflns_number_total             9839
_reflns_threshold_expression     I>=2u(I)
_cod_data_source_file            c4ra02751e2.cif
_cod_data_source_block           FHMS-24
_cod_database_code               7235661
_chemical_oxdiff_usercomment     '23 JULY 2013'
_reflns_odcompleteness_completeness 99.80
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     26.32
_olex2_refinement_description
;
;
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,y+1/2,-z+1/2
3 -x,-y,-z
4 x,-y-1/2,z-1/2
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
C1 C -0.1346(13) 1.082(2) 0.0714(12) 0.017(5) Uiso 1.000000
C2 C -0.0762(11) 1.0100(17) 0.0666(10) 0.006(4) Uiso 1.000000
O1 O 0.4948(8) 0.8710(12) 0.4328(8) 0.011(3) Uiso 1.000000
O2 O 0.4239(8) 0.5744(13) 0.2246(8) 0.012(3) Uiso 1.000000
O3 O 0.2917(8) 0.5650(13) 0.4100(8) 0.013(3) Uiso 1.000000
O4 O 0.4429(8) 0.7462(12) 0.3192(8) 0.010(3) Uiso 1.000000
O5 O 0.3483(8) 0.5953(12) 0.3090(8) 0.010(3) Uiso 1.000000
O6 O 0.3766(8) 0.7389(13) 0.4090(8) 0.012(3) Uiso 1.000000
O7 O 0.4182(7) 0.9531(11) 0.3046(7) 0.006(3) Uiso 1.000000
O8 O 0.3831(8) 0.7876(12) 0.1877(8) 0.011(3) Uiso 1.000000
O9 O 0.2858(8) 0.6469(12) 0.1765(7) 0.007(3) Uiso 1.000000
O10 O 0.2067(8) 0.6348(13) 0.2816(8) 0.012(3) Uiso 1.000000
O11 O 0.2376(8) 0.7709(12) 0.3812(7) 0.010(3) Uiso 1.000000
O12 O 0.3527(8) 0.9450(12) 0.3923(7) 0.007(3) Uiso 1.000000
O13 O 0.3101(7) 0.7951(12) 0.2853(7) 0.006(3) Uiso 1.000000
O14 O 0.1163(8) 0.8415(12) 0.4065(7) 0.009(3) Uiso 1.000000
O15 O 0.2312(8) 0.9735(12) 0.4103(7) 0.009(3) Uiso 1.000000
O16 O 0.3240(9) 1.1457(13) 0.4375(8) 0.016(3) Uiso 1.000000
O17 O 0.3285(8) 1.1004(12) 0.3076(8) 0.010(3) Uiso 1.000000
O18 O 0.4441(8) 1.1631(12) 0.2717(7) 0.009(3) Uiso 1.000000
O19 O 0.4031(8) 0.9951(13) 0.1781(8) 0.011(3) Uiso 1.000000
O20 O 0.3785(9) 0.8671(13) 0.0632(8) 0.016(3) Uiso 1.000000
O21 O 0.2599(8) 0.7985(12) 0.0893(8) 0.010(3) Uiso 1.000000
O22 O 0.2024(8) 0.5996(13) 0.0438(8) 0.014(3) Uiso 1.000000
O23 O 0.1451(7) 0.6098(11) 0.1456(7) 0.005(3) Uiso 1.000000
O24 O 0.0651(9) 0.5796(13) 0.2280(8) 0.014(3) Uiso 1.000000
O25 O 0.1148(7) 0.7817(12) 0.2805(7) 0.006(3) Uiso 1.000000
O26 O 0.2147(7) 0.9421(12) 0.2823(7) 0.006(3) Uiso 1.000000
O27 O 0.2830(7) 0.9488(12) 0.1940(7) 0.006(3) Uiso 1.000000
O28 O 0.1859(7) 0.7977(11) 0.1830(7) 0.006(3) Uiso 1.000000
O29 O 0.1026(8) 0.9892(12) 0.3073(7) 0.008(3) Uiso 1.000000
O30 O 0.2018(8) 1.1331(13) 0.3215(8) 0.012(3) Uiso 1.000000
O31 O 0.3088(8) 1.1442(12) 0.1767(7) 0.007(3) Uiso 1.000000
O32 O 0.2781(8) 1.0069(12) 0.0765(7) 0.007(3) Uiso 1.000000
O33 O 0.1141(8) 0.7605(13) 0.0478(8) 0.012(3) Uiso 1.000000
O34 O 0.0430(8) 0.7556(12) 0.1475(7) 0.008(3) Uiso 1.000000
O35 O 0.1461(8) 0.9827(13) 0.0862(8) 0.012(3) Uiso 1.000000
O36 O 0.0763(8) 0.9808(13) 0.1741(8) 0.012(3) Uiso 1.000000
O37 O 0.1839(8) 1.1169(12) 0.1901(7) 0.008(3) Uiso 1.000000
O38 O 0.0675(8) 1.1763(12) 0.2286(8) 0.011(3) Uiso 1.000000
O39 O 0.1859(8) 1.1807(12) 0.0604(7) 0.009(3) Uiso 1.000000
O40 O 0.0329(7) 0.9557(12) -0.0379(7) 0.006(3) Uiso 1.000000
O41 O -0.0411(8) 0.7797(12) -0.0023(8) 0.010(3) Uiso 1.000000
O42 O -0.0672(8) 0.9206(12) 0.0934(8) 0.011(3) Uiso 1.000000
O43 O -0.1733(9) 0.8967(14) 0.1810(9) 0.020(4) Uiso 1.000000
O44 O 0.4571(12) 0.9004(19) 0.5831(11) 0.040(5) Uiso 1.000000
O45 O 0.3946(10) 0.3858(16) 0.3212(10) 0.026(4) Uiso 1.000000
O46 O 0.0776(12) 1.3747(19) -0.0989(11) 0.040(5) Uiso 1.000000
O47 O 0.4707(17) 1.293(3) 0.4467(16) 0.070(8) Uiso 1.000000
O48 O 0.3161(9) 1.3762(14) 0.4817(8) 0.017(4) Uiso 1.000000
O49 O 0.4704(10) 1.4057(16) 0.5930(10) 0.028(4) Uiso 1.000000
O50 O 0.3690(11) 1.1998(17) 0.6124(10) 0.031(5) Uiso 1.000000
O51 O 0.2298(10) 0.3864(16) 0.0317(10) 0.027(4) Uiso 1.000000
O52 O 0.1637(12) 0.3975(18) 0.1293(11) 0.037(5) Uiso 1.000000
O53 O -0.0323(11) 0.6928(16) -0.1170(10) 0.029(4) Uiso 1.000000
O54 O 0.2563(11) 1.3191(16) 0.2497(10) 0.029(4) Uiso 1.000000
O55 O 0.0519(7) 0.9582(11) 0.4799(7) 0.005(3) Uiso 1.000000
Na1 Na 0.4528(7) 0.9459(10) -0.0117(6) 0.038(3) Uiso 1.000000
Na2 Na 0.4071(6) 1.2561(9) 0.5221(6) 0.029(2) Uiso 1.000000
Si1 Si 0.2471(3) 0.8690(5) 0.2356(3) 0.0086(11) Uani 1.000000
K1 K -0.0275(3) 0.8814(4) 0.2315(2) 0.0137(10) Uani 1.000000
K2 K 0.3259(3) 0.8393(5) 0.5096(3) 0.0191(11) Uani 1.000000
K3 K 0.4712(3) 0.3664(4) 0.2379(3) 0.0164(10) Uani 1.000000
K4 K 0.1900(3) 1.2378(5) -0.0685(3) 0.0287(13) Uani 1.000000
Ho1 Ho 0.04531(5) 0.88910(7) 0.07303(5) 0.00625(19) Uani 1.000000
W1 W 0.41378(4) 0.84846(7) 0.36974(4) 0.00664(17) Uani 1.000000
W2 W 0.37084(4) 0.66979(7) 0.24029(4) 0.00680(18) Uani 1.000000
W3 W 0.28860(4) 0.66285(7) 0.35327(4) 0.00708(18) Uani 1.000000
W4 W 0.16201(4) 0.87275(7) 0.35426(4) 0.00618(17) Uani 1.000000
W5 W 0.28478(4) 1.05997(7) 0.37054(4) 0.00690(18) Uani 1.000000
W6 W 0.37695(4) 1.07162(7) 0.24654(4) 0.00612(17) Uani 1.000000
W7 W 0.33825(4) 0.89226(7) 0.12107(4) 0.00636(17) Uani 1.000000
W8 W 0.19277(4) 0.69653(7) 0.09917(4) 0.00622(17) Uani 1.000000
W9 W 0.11189(4) 0.68137(6) 0.20989(4) 0.00561(17) Uani 1.000000
W10 W 0.21556(4) 1.07642(7) 0.11728(4) 0.00590(17) Uani 1.000000
W11 W 0.12499(4) 1.07099(7) 0.23875(4) 0.00618(17) Uani 1.000000
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_source
_atom_type_scat_dispersion_source
C 0.00347 0.00161 2.31000 1.02000 1.58860 0.86500 20.84390 10.20750 0.56870
51.65120 0.215599998832
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Na 0.03665 0.02467 4.76260 3.17360 1.26740 1.11280 3.28500 8.84220 0.31360
129.42400 0.675999999046
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
K 0.21174 0.26561 8.21860 7.43980 1.05190 0.86590 12.79490 0.77480 213.18700
41.68410 1.42279994488
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
O 0.01158 0.00611 3.04850 2.28680 1.54630 0.86700 13.27710 5.70110 0.32390
32.90890 0.250800013542
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Si 0.08192 0.07060 6.29150 3.03530 1.98910 1.54100 2.43860 32.33370 0.67850
81.69370 1.14069998264
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Ho -0.01807 5.00960 26.90490 17.29400 14.55830 3.63837 2.07051 0.19794 11.44070
92.65660 4.56795978546
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
W -0.66836 6.76498 29.08180 15.43000 14.43270 5.11982 1.72029 9.22590 0.32170
57.05600 9.88749980927
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O40 C2 C1 119.6(19) 3_575 .
O42 C2 C1 120.2(19) . .
O42 C2 O40 120.1(19) . 3_575
Ho1 C2 C1 172.5(15) . .
Ho1 C2 O40 59.8(10) . 3_575
Ho1 C2 O42 60.4(11) . .
W1 O1 Na2 126.9(8) . 3_676
W2 O2 K3 149.3(8) . .
W1 O4 K3 103.0(6) . 2_655
W2 O4 K3 105.7(6) . 2_655
W2 O4 W1 121.0(8) . .
W3 O5 W2 119.7(8) . .
W1 O6 K2 106.8(6) . .
W3 O6 K2 100.0(6) . .
W3 O6 W1 119.9(8) . .
W1 O7 K3 101.1(6) . 2_655
W6 O7 K3 107.6(6) . 2_655
W6 O7 W1 150.2(8) . .
W2 O8 K3 104.9(6) . 2_655
W7 O8 K3 106.2(6) . 2_655
W7 O8 W2 146.9(9) . .
W8 O9 W2 153.0(9) . .
W9 O10 W3 151.6(9) . .
W3 O11 K2 106.9(6) . .
W4 O11 K2 104.3(6) . .
W4 O11 W3 147.0(8) . .
W1 O12 K2 103.7(6) . .
W5 O12 K2 102.3(6) . .
W5 O12 W1 152.1(8) . .
W1 O13 Si1 128.0(8) . .
W2 O13 Si1 121.1(8) . .
W2 O13 W1 93.0(5) . .
W3 O13 Si1 122.4(8) . .
W3 O13 W1 92.7(5) . .
W3 O13 W2 90.0(5) . .
W4 O15 K2 102.0(6) . .
W5 O15 K2 109.1(6) . .
W5 O15 W4 119.8(8) . .
K4 O16 Na2 97.1(6) 4_586 .
W5 O16 Na2 164.0(10) . .
W5 O16 K4 97.3(7) . 4_586
W6 O17 W5 153.2(9) . .
W6 O18 K3 138.6(8) . 1_565
W6 O19 K3 102.7(6) . 2_655
W7 O19 K3 104.3(6) . 2_655
W7 O19 W6 119.7(8) . .
K2 O20 Na1 107.7(6) 4_575 .
W7 O20 Na1 147.1(9) . .
W7 O20 K2 104.3(7) . 4_575
W7 O21 K2 94.9(6) . 4_575
W8 O21 K2 97.7(6) . 4_575
W8 O21 W7 154.8(9) . .
W8 O22 K2 106.4(7) . 4_575
W9 O23 W8 116.4(7) . .
W9 O24 K1 163.0(9) . 2_545
W4 O25 K1 99.9(6) . .
W9 O25 K1 104.2(6) . .
W9 O25 W4 153.6(8) . .
W4 O26 Si1 123.4(8) . .
W5 O26 Si1 124.3(8) . .
W5 O26 W4 90.3(5) . .
W11 O26 Si1 124.4(8) . .
W11 O26 W4 93.1(5) . .
W11 O26 W5 91.9(5) . .
W6 O27 Si1 124.6(8) . .
W7 O27 Si1 124.4(8) . .
W7 O27 W6 91.4(5) . .
W10 O27 Si1 122.0(8) . .
W10 O27 W6 92.5(5) . .
W10 O27 W7 92.9(5) . .
W8 O28 Si1 128.6(8) . .
W9 O28 Si1 126.2(8) . .
W9 O28 W8 93.1(5) . .
W4 O29 K1 101.6(6) . .
W11 O29 K1 103.8(6) . .
W11 O29 W4 121.4(8) . .
W5 O30 K4 98.2(6) . 4_586
W11 O30 K4 130.4(7) . 4_586
W11 O30 W5 122.9(8) . .
W10 O31 W6 122.7(8) . .
W10 O32 W7 121.1(7) . .
W8 O33 Ho1 131.2(8) . .
Ho1 O34 K1 97.9(5) . .
W9 O34 K1 103.9(6) . .
W9 O34 Ho1 133.0(8) . .
W10 O35 Ho1 160.8(9) . .
Ho1 O36 K1 99.2(5) . .
W11 O36 K1 103.3(6) . .
W11 O36 Ho1 157.5(9) . .
W11 O37 W10 142.0(8) . .
W11 O38 K1 152.6(8) . 2
W10 O39 K4 137.2(8) . .
Ho1 O40 C2 93.1(12) 3_575 3_575
Ho1 O40 C2 135.3(13) . 3_575
K1 O42 C2 125.3(13) . .
K4 O42 C2 122.2(13) 3_575 .
K4 O42 K1 88.9(5) 3_575 .
Ho1 O42 C2 93.6(12) . .
Ho1 O42 K1 102.0(5) . .
Ho1 O42 K4 126.3(6) . 3_575
K4 O43 K1 94.5(6) 3_575 .
Na2 O47 Na1 98.8(12) . 2_655
K4 O48 Na2 107.4(7) 4_586 .
Na2 O49 Na1 92.7(7) . 2_655
K3 O50 Na2 119.9(8) 4_576 .
O47 Na1 O20 76.1(9) 2_645 .
O49 Na1 O20 147.7(8) 2_645 .
O49 Na1 O47 80.2(9) 2_645 2_645
Na1 Na1 O20 133.6(9) 3_675 .
Na1 Na1 O47 92.3(10) 3_675 2_645
Na1 Na1 O49 68.4(7) 3_675 2_645
O16 Na2 O1 99.3(7) . 3_676
O47 Na2 O1 81.0(9) . 3_676
O47 Na2 O16 90.9(9) . .
O48 Na2 O1 179.0(8) . 3_676
O48 Na2 O16 81.6(7) . .
O48 Na2 O47 99.4(10) . .
O49 Na2 O1 95.3(7) . 3_676
O49 Na2 O16 165.0(8) . .
O49 Na2 O47 88.3(10) . .
O49 Na2 O48 83.8(7) . .
O50 Na2 O1 86.3(7) . 3_676
O50 Na2 O16 94.8(7) . .
O50 Na2 O47 166.8(11) . .
O50 Na2 O48 93.2(8) . .
O50 Na2 O49 89.2(8) . .
O26 Si1 O13 108.7(8) . .
O27 Si1 O13 107.8(8) . .
O27 Si1 O26 108.2(8) . .
O28 Si1 O13 110.9(8) . .
O28 Si1 O26 111.1(8) . .
O28 Si1 O27 110.1(8) . .
O25 K1 O24 126.7(5) . 2
O29 K1 O24 72.6(5) . 2
O29 K1 O25 55.3(4) . .
O34 K1 O24 149.0(5) . 2
O34 K1 O25 52.9(4) . .
O34 K1 O29 93.0(4) . .
O36 K1 O24 92.7(5) . 2
O36 K1 O25 66.4(4) . .
O36 K1 O29 53.7(4) . .
O36 K1 O34 57.5(4) . .
O38 K1 O24 124.6(5) 2_545 2
O38 K1 O25 81.4(4) 2_545 .
O38 K1 O29 123.1(5) 2_545 .
O38 K1 O34 86.3(4) 2_545 .
O38 K1 O36 141.3(5) 2_545 .
O42 K1 O24 98.6(5) . 2
O42 K1 O25 109.2(4) . .
O42 K1 O29 111.6(5) . .
O42 K1 O34 60.6(4) . .
O42 K1 O36 59.5(4) . .
O42 K1 O38 116.9(5) . 2_545
O43 K1 O24 72.2(5) . 2
O43 K1 O25 158.9(5) . .
O43 K1 O29 144.8(5) . .
O43 K1 O34 117.2(5) . .
O43 K1 O36 127.3(5) . .
O43 K1 O38 79.1(5) . 2_545
O43 K1 O42 73.0(5) . .
O53 K1 O24 82.0(5) 4_576 2
O53 K1 O25 84.0(5) 4_576 .
O53 K1 O29 85.8(5) 4_576 .
O53 K1 O34 125.2(5) 4_576 .
O53 K1 O36 138.5(5) 4_576 .
O53 K1 O38 51.5(5) 4_576 2_545
O53 K1 O42 162.0(5) 4_576 .
O53 K1 O43 90.3(5) 4_576 .
O11 K2 O6 55.5(4) . .
O12 K2 O6 52.8(4) . .
O12 K2 O11 65.2(4) . .
O15 K2 O6 92.2(4) . .
O15 K2 O11 55.9(4) . .
O15 K2 O12 53.1(4) . .
O20 K2 O6 73.8(5) 4_576 .
O20 K2 O11 96.9(5) 4_576 .
O20 K2 O12 125.0(5) 4_576 .
O20 K2 O15 152.2(5) 4_576 .
O21 K2 O6 118.7(5) 4_576 .
O21 K2 O11 96.1(5) 4_576 .
O21 K2 O12 161.2(4) 4_576 .
O21 K2 O15 116.2(5) 4_576 .
O21 K2 O20 55.6(4) 4_576 4_576
O22 K2 O6 146.2(5) 4_576 .
O22 K2 O11 90.8(5) 4_576 .
O22 K2 O12 119.7(5) 4_576 .
O22 K2 O15 67.4(4) 4_576 .
O22 K2 O20 111.6(5) 4_576 4_576
O22 K2 O21 55.9(4) 4_576 4_576
O44 K2 O6 91.3(6) . .
O44 K2 O11 144.6(6) . .
O44 K2 O12 85.7(6) . .
O44 K2 O15 121.8(6) . .
O44 K2 O20 83.3(6) . 4_576
O44 K2 O21 112.4(6) . 4_576
O44 K2 O22 122.2(6) . 4_576
O4 K3 O2 134.1(5) 2_645 .
O7 K3 O2 83.3(4) 2_645 .
O7 K3 O4 55.1(4) 2_645 2_645
O8 K3 O2 127.7(5) 2_645 .
O8 K3 O4 54.2(4) 2_645 2_645
O8 K3 O7 64.4(4) 2_645 2_645
O18 K3 O2 144.4(5) 1_545 .
O18 K3 O4 79.5(5) 1_545 2_645
O18 K3 O7 132.4(5) 1_545 2_645
O18 K3 O8 78.4(4) 1_545 2_645
O19 K3 O2 74.6(5) 2_645 .
O19 K3 O4 91.7(4) 2_645 2_645
O19 K3 O7 53.0(4) 2_645 2_645
O19 K3 O8 53.2(4) 2_645 2_645
O19 K3 O18 123.4(5) 2_645 1_545
O45 K3 O2 74.3(5) . .
O45 K3 O4 151.6(6) . 2_645
O45 K3 O7 146.8(5) . 2_645
O45 K3 O8 111.4(5) . 2_645
O45 K3 O18 73.2(5) . 1_545
O45 K3 O19 96.9(5) . 2_645
O50 K3 O2 94.3(6) 4_575 .
O50 K3 O4 78.3(5) 4_575 2_645
O50 K3 O7 101.8(5) 4_575 2_645
O50 K3 O8 130.4(5) 4_575 2_645
O50 K3 O18 79.9(5) 4_575 1_545
O50 K3 O19 152.9(5) 4_575 2_645
O50 K3 O45 103.9(6) 4_575 .
O30 K4 O16 56.1(4) 4_585 4_585
O39 K4 O16 114.0(5) . 4_585
O39 K4 O30 160.4(5) . 4_585
O42 K4 O16 166.1(5) 3_575 4_585
O42 K4 O30 120.9(5) 3_575 4_585
O42 K4 O39 73.0(4) 3_575 .
O43 K4 O16 99.7(5) 3_575 4_585
O43 K4 O30 71.9(5) 3_575 4_585
O43 K4 O39 127.8(5) 3_575 .
O43 K4 O42 67.4(5) 3_575 3_575
O46 K4 O16 110.5(6) . 4_585
O46 K4 O30 75.5(6) . 4_585
O46 K4 O39 95.0(6) . .
O46 K4 O42 79.9(6) . 3_575
O46 K4 O43 109.6(6) . 3_575
O48 K4 O16 63.8(5) 4_585 4_585
O48 K4 O30 106.0(5) 4_585 4_585
O48 K4 O39 80.3(5) 4_585 .
O48 K4 O42 107.3(5) 4_585 3_575
O48 K4 O43 80.4(5) 4_585 3_575
O48 K4 O46 169.6(7) 4_585 .
O51 K4 O16 67.6(5) 1_565 4_585
O51 K4 O30 98.5(5) 1_565 4_585
O51 K4 O39 62.2(5) 1_565 .
O51 K4 O42 125.4(5) 1_565 3_575
O51 K4 O43 167.2(6) 1_565 3_575
O51 K4 O46 74.9(6) 1_565 .
O51 K4 O48 94.7(6) 1_565 4_585
O33 Ho1 C2 159.9(6) . .
O34 Ho1 C2 101.7(5) . .
O34 Ho1 O33 78.4(5) . .
O35 Ho1 C2 116.0(6) . .
O35 Ho1 O33 79.4(6) . .
O35 Ho1 O34 121.6(5) . .
O36 Ho1 C2 74.0(6) . .
O36 Ho1 O33 125.1(5) . .
O36 Ho1 O34 78.7(5) . .
O36 Ho1 O35 71.7(5) . .
O40 Ho1 C2 27.1(5) 3_575 .
O40 Ho1 C2 88.3(5) . .
O40 Ho1 O33 149.5(5) 3_575 .
O40 Ho1 O33 83.7(5) . .
O40 Ho1 O34 128.5(5) 3_575 .
O40 Ho1 O34 153.0(5) . .
O40 Ho1 O35 94.0(5) 3_575 .
O40 Ho1 O35 73.9(5) . .
O40 Ho1 O36 128.4(5) . .
O40 Ho1 O36 79.3(5) 3_575 .
O41 Ho1 C2 82.3(6) . .
O41 Ho1 O33 77.9(5) . .
O41 Ho1 O34 81.0(5) . .
O41 Ho1 O35 143.5(5) . .
O41 Ho1 O36 144.6(5) . .
O41 Ho1 O40 91.4(5) . 3_575
O41 Ho1 O40 75.5(5) . .
O42 Ho1 C2 26.0(6) . .
O42 Ho1 O33 143.9(5) . .
O42 Ho1 O34 76.3(5) . .
O42 Ho1 O35 136.2(5) . .
O42 Ho1 O36 74.2(5) . .
O42 Ho1 O40 108.7(5) . .
O42 Ho1 O40 53.0(5) . 3_575
O42 Ho1 O41 73.1(5) . .
O4 W1 O1 98.8(7) . .
O6 W1 O1 101.2(7) . .
O6 W1 O4 89.7(7) . .
O7 W1 O1 99.7(7) . .
O7 W1 O4 88.1(6) . .
O7 W1 O6 159.1(6) . .
O12 W1 O1 102.5(7) . .
O12 W1 O4 158.6(6) . .
O12 W1 O6 88.4(6) . .
O12 W1 O7 86.1(6) . .
O13 W1 O1 172.4(6) . .
O13 W1 O4 74.9(6) . .
O13 W1 O6 74.8(6) . .
O13 W1 O7 84.6(5) . .
O13 W1 O12 84.0(6) . .
O4 W2 O2 100.4(7) . .
O5 W2 O2 97.3(7) . .
O5 W2 O4 84.5(6) . .
O8 W2 O2 102.7(7) . .
O8 W2 O4 84.5(6) . .
O8 W2 O5 158.6(6) . .
O9 W2 O2 103.6(7) . .
O9 W2 O4 156.0(6) . .
O9 W2 O5 94.2(6) . .
O9 W2 O8 88.5(7) . .
O13 W2 O2 168.6(6) . .
O13 W2 O4 71.0(5) . .
O13 W2 O5 74.7(6) . .
O13 W2 O8 84.4(6) . .
O13 W2 O9 85.4(6) . .
O5 W3 O3 98.1(7) . .
O6 W3 O3 97.4(7) . .
O6 W3 O5 85.8(6) . .
O10 W3 O3 103.8(7) . .
O10 W3 O5 92.6(7) . .
O10 W3 O6 158.7(7) . .
O11 W3 O3 101.1(7) . .
O11 W3 O5 160.0(6) . .
O11 W3 O6 86.2(6) . .
O11 W3 O10 88.2(7) . .
O13 W3 O3 168.1(6) . .
O13 W3 O5 75.1(6) . .
O13 W3 O6 72.6(6) . .
O13 W3 O10 86.5(6) . .
O13 W3 O11 85.0(6) . .
O14 W4 O11 101.6(7) . .
O15 W4 O11 86.4(6) . .
O15 W4 O14 100.9(7) . .
O25 W4 O11 87.3(6) . .
O25 W4 O14 99.3(7) . .
O25 W4 O15 159.7(6) . .
O26 W4 O11 87.2(6) . .
O26 W4 O14 170.5(6) . .
O26 W4 O15 75.9(6) . .
O26 W4 O25 84.5(6) . .
O29 W4 O11 160.8(6) . .
O29 W4 O14 97.5(7) . .
O29 W4 O15 89.6(6) . .
O29 W4 O25 90.0(6) . .
O29 W4 O26 73.6(6) . .
O15 W5 O12 85.7(6) . .
O16 W5 O12 101.2(7) . .
O16 W5 O15 99.4(7) . .
O17 W5 O12 84.7(6) . .
O17 W5 O15 157.6(6) . .
O17 W5 O16 102.2(7) . .
O26 W5 O12 83.8(5) . .
O26 W5 O15 73.8(6) . .
O26 W5 O16 171.4(6) . .
O26 W5 O17 85.1(6) . .
O30 W5 O12 157.0(6) . .
O30 W5 O15 89.7(7) . .
O30 W5 O16 101.7(7) . .
O30 W5 O17 91.2(7) . .
O30 W5 O26 73.4(6) . .
O17 W6 O7 85.8(6) . .
O18 W6 O7 102.2(7) . .
O18 W6 O17 101.3(7) . .
O19 W6 O7 85.3(6) . .
O19 W6 O17 158.1(7) . .
O19 W6 O18 100.2(7) . .
O27 W6 O7 83.3(5) . .
O27 W6 O17 86.0(6) . .
O27 W6 O18 171.1(6) . .
O27 W6 O19 73.1(6) . .
O31 W6 O7 156.6(6) . .
O31 W6 O17 91.8(6) . .
O31 W6 O18 101.1(7) . .
O31 W6 O19 88.5(6) . .
O31 W6 O27 73.3(6) . .
O19 W7 O8 88.1(6) . .
O20 W7 O8 100.2(7) . .
O20 W7 O19 100.6(7) . .
O21 W7 O8 86.9(7) . .
O21 W7 O19 159.4(6) . .
O21 W7 O20 100.0(7) . .
O27 W7 O8 86.4(6) . .
O27 W7 O19 75.7(6) . .
O27 W7 O20 172.5(7) . .
O27 W7 O21 84.0(6) . .
O32 W7 O8 160.3(6) . .
O32 W7 O19 88.2(6) . .
O32 W7 O20 99.6(7) . .
O32 W7 O21 89.8(6) . .
O32 W7 O27 73.9(6) . .
O21 W8 O9 79.5(6) . .
O22 W8 O9 91.9(7) . .
O22 W8 O21 98.6(7) . .
O23 W8 O9 84.3(6) . .
O23 W8 O21 157.4(6) . .
O23 W8 O22 97.6(7) . .
O28 W8 O9 80.9(5) . .
O28 W8 O21 86.7(6) . .
O28 W8 O22 170.1(6) . .
O28 W8 O23 75.1(5) . .
O33 W8 O9 166.8(6) . .
O33 W8 O21 97.9(7) . .
O33 W8 O22 101.3(7) . .
O33 W8 O23 94.3(7) . .
O33 W8 O28 86.1(6) . .
O23 W9 O10 85.6(6) . .
O24 W9 O10 93.5(7) . .
O24 W9 O23 99.0(7) . .
O25 W9 O10 81.5(6) . .
O25 W9 O23 156.8(6) . .
O25 W9 O24 101.0(7) . .
O28 W9 O10 81.5(6) . .
O28 W9 O23 73.4(5) . .
O28 W9 O24 171.1(7) . .
O28 W9 O25 85.6(6) . .
O34 W9 O10 163.8(6) . .
O34 W9 O23 95.6(6) . .
O34 W9 O24 102.3(7) . .
O34 W9 O25 91.6(6) . .
O34 W9 O28 83.3(6) . .
O31 W10 O27 71.5(5) . .
O32 W10 O27 72.0(5) . .
O32 W10 O31 82.3(6) . .
O35 W10 O27 89.1(6) . .
O35 W10 O31 160.4(6) . .
O35 W10 O32 94.6(7) . .
O37 W10 O27 84.6(6) . .
O37 W10 O31 83.5(6) . .
O37 W10 O32 155.5(6) . .
O37 W10 O35 92.0(7) . .
O39 W10 O27 165.9(6) . .
O39 W10 O31 97.1(6) . .
O39 W10 O32 98.9(6) . .
O39 W10 O35 102.5(7) . .
O39 W10 O37 102.7(7) . .
O29 W11 O26 71.9(6) . .
O30 W11 O26 71.8(6) . .
O30 W11 O29 82.6(6) . .
O36 W11 O26 89.7(6) . .
O36 W11 O29 91.2(7) . .
O36 W11 O30 161.5(7) . .
O37 W11 O26 83.4(6) . .
O37 W11 O29 154.9(6) . .
O37 W11 O30 85.2(6) . .
O37 W11 O36 93.5(7) . .
O38 W11 O26 165.0(6) . .
O38 W11 O29 100.5(7) . .
O38 W11 O30 94.7(7) . .
O38 W11 O36 103.6(7) . .
O38 W11 O37 102.3(7) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
C1 C2 1.51(3) .
C2 O40 1.30(2) 3_575
C2 O42 1.25(3) .
C2 Ho1 2.84(2) .
O1 Na2 2.459(19) 3_676
O1 W1 1.725(15) .
O2 K3 2.773(17) .
O2 W2 1.715(16) .
O3 W3 1.705(16) .
O4 K3 2.860(16) 2_655
O4 W1 1.892(15) .
O4 W2 2.024(15) .
O5 W2 1.909(15) .
O5 W3 1.954(15) .
O6 K2 2.939(16) .
O6 W1 1.895(16) .
O6 W3 1.991(15) .
O7 K3 2.886(15) 2_655
O7 W1 1.929(14) .
O7 W6 1.927(14) .
O8 K3 2.964(16) 2_655
O8 W2 1.921(15) .
O8 W7 1.909(15) .
O9 W2 1.787(14) .
O9 W8 2.098(14) .
O10 W3 1.835(15) .
O10 W9 2.057(15) .
O11 K2 2.800(16) .
O11 W3 1.919(15) .
O11 W4 1.916(15) .
O12 K2 3.017(15) .
O12 W1 1.904(14) .
O12 W5 1.934(15) .
O13 Si1 1.624(15) .
O13 W1 2.313(14) .
O13 W2 2.387(14) .
O13 W3 2.337(14) .
O14 W4 1.708(15) .
O15 K2 2.841(16) .
O15 W4 1.947(15) .
O15 W5 1.920(15) .
O16 Na2 2.41(2) .
O16 K4 3.030(18) 4_586
O16 W5 1.732(17) .
O17 W5 1.899(15) .
O17 W6 1.900(15) .
O18 K3 2.770(16) 1_565
O18 W6 1.712(15) .
O19 K3 3.002(16) 2_655
O19 W6 1.954(15) .
O19 W7 1.931(15) .
O20 Na1 2.71(2) .
O20 K2 2.890(18) 4_575
O20 W7 1.712(16) .
O21 K2 3.027(16) 4_575
O21 W7 1.893(15) .
O21 W8 1.928(15) .
O22 K2 2.917(17) 4_575
O22 W8 1.748(16) .
O23 W8 1.931(14) .
O23 W9 1.930(14) .
O24 K1 2.832(17) 2_545
O24 W9 1.711(16) .
O25 K1 2.957(15) .
O25 W4 1.897(14) .
O25 W9 1.940(14) .
O26 Si1 1.639(15) .
O26 W4 2.305(14) .
O26 W5 2.412(14) .
O26 W11 2.362(14) .
O27 Si1 1.657(15) .
O27 W6 2.393(14) .
O27 W7 2.301(14) .
O27 W10 2.347(14) .
O28 Si1 1.611(15) .
O28 W8 2.223(14) .
O28 W9 2.297(14) .
O29 K1 2.882(16) .
O29 W4 1.933(15) .
O29 W11 1.952(15) .
O30 K4 2.911(17) 4_586
O30 W5 1.867(16) .
O30 W11 2.037(15) .
O31 W6 1.862(14) .
O31 W10 2.039(14) .
O32 W7 1.908(15) .
O32 W10 1.960(14) .
O33 Ho1 2.312(16) .
O33 W8 1.765(16) .
O34 K1 3.068(15) .
O34 Ho1 2.314(15) .
O34 W9 1.801(15) .
O35 Ho1 2.274(16) .
O35 W10 1.771(16) .
O36 K1 3.025(16) .
O36 Ho1 2.309(15) .
O36 W11 1.782(16) .
O37 W10 1.924(15) .
O37 W11 1.907(15) .
O38 K1 2.922(16) 2
O38 W11 1.724(15) .
O39 K4 2.838(16) .
O39 W10 1.738(15) .
O40 Ho1 2.412(14) .
O40 Ho1 2.457(14) 3_575
O41 Ho1 2.346(15) .
O42 K1 2.778(16) .
O42 K4 3.072(17) 3_575
O42 Ho1 2.474(15) .
O43 K1 2.746(18) .
O43 K4 2.839(19) 3_575
O44 K2 2.66(2) .
O45 K3 2.72(2) .
O46 K4 2.73(2) .
O47 Na1 2.54(3) 2_655
O47 Na2 2.41(3) .
O48 Na2 2.30(2) .
O48 K4 2.779(18) 4_586
O49 Na1 2.72(2) 2_655
O49 Na2 2.47(2) .
O50 Na2 2.39(2) .
O50 K3 2.85(2) 4_576
O51 K4 2.73(2) 1_545
O53 K1 3.36(2) 4_575
Na1 Na1 2.25(3) 3_675
